Symmetryoperations, point groups, space groups and crystal structure


 Geraldine Nichols
 1 years ago
 Views:
Transcription
1 1 Symmetryoperations, point groups, space groups and crystal structure KJ/MV 210 Helmer Fjellvåg, Department of Chemistry, University of Oslo 1994 This compendium replaces chapter 5.3 and 6 in West. Sections not part of the curriculum are enclosed in asterisks (*). It is recommended that the textbooks of West and Jastrzebski are used as supplementary reading material, with special emphasis on illustrative examples. In this compendium illustrative examples (in italics) have been chosen from close packed structures. A few symbols and synonyms are given in Norwegian as information. The compendium contains exercises which will not be explained in the classes. It is recommended to work through the exercises while reading this compendium. Introduction. Condensed phases may be liquids as well as solids. There are fundamental differences between liquids and solids regarding the longrange distribution of atoms. While liquids have long range disorder in a large scale, solids are mainly ordered, i.e. there is regularity in the repetition of structural fragments (atoms and/or groups of atoms) in the 3 dimensional material. Surfaces of solid materials are often somewhat differently organized than the bulk (i.e. the inner part of the material). The atomic (structural) arrangement near the surface will often be different from the bulk arrangement due to surface reconstruction in order to minimize the energy loss associated with complete chemical bonding in all actual directions. Liquids are disordered in bulk, but they often have an ordered surface structure. Solids do not need to display systematic longrange order, i.e. to be crystalline. Some phases can be prepared as amorphous materials, e.g. glasses. They may be made crystallized by a suitable temperature treatment. A few phases exist which are only known in an amorphous state. In order to simplify the description of symmetry relations in atomic arrangements (i.e. the appearance of a structure fragment, molecule or complex) symmetry operations are used. Symmetryoperations like mirroring and rotation are known from everydaylife. If one wishes to describe how structure fragments are repeated (translated) through a solid compound, symmetryoperations which include translation must be used in addition. Symmetrydescriptions of given isolated objects are also known from everydaylife, e.g. a lump of sugar, a dice, a wheel (with an nfold rotation axes for n spokes equally distributed) or a pyramid (with fourfold rotation axis perpendicular to the basis plan).
2 This compendium does not intend to give complete introduction to the basics of symmetry descriptions of solids. That is not the objective of this part of KJMV 210. The text is not written in order to give the reader a perfect and full understanding of crystallography. Instead it will give a simplified picture of the field. The intension of the compendium is to provide a basic knowledge of central issues, so that the reader will be able to draw different structures based on published structural data and available references (International Tables of Crystallography). This will be very useful in later courses concerned with properties of inorganic materials. It is important to realise that there is a close connection between atomic arrangements (structure, chemical bonding) and chemical and physical properties. The chosen examples in the compendium are related to close packing of atoms. The reader is recommended to carefully work through the examples. The unit cell. In the crystalline state there are rules for how structural elements are repeated through the solid. One can identify structural fragments that form the smallest repeating units; by repeating these in 3 dimensions they build the whole material. One can think of the smallest repeating unit as described inside a box. By stacking of the boxes in 3 dimensions a complete description of the structure of the solid material is obtained. Such a box is called a unit cell (enhetscelle). The box is defined by 3 vectors, t 1, t 2 and t 3 [with unit cell volume V = t 1 (t 2 x t 3 )]. The vectors are not necessarily orthogonal. As a starting point there are no conditions on the 3 angles between the vectors, α, β and γ. (i.e. they are not restricted in any way, e.g. to be 90 ). When describing the structure of a solid material in the scientific literature, relevant data for the crystallographic unit cell are given. The unit cell is given by the length of the three axes, a, b and c (unit cell dimensions, unit cell parameters, cell edges; i.e. the lengths of the vectors t 1, t 2 and t 3 ) and the angles α, β and γ. Definition of the angles relative to the axes (t 1, t 2 and t 3 or equivalent a, b and c) is shown in Figure 1. In order to describe the atomic arrangement, one has in addition to defining the shape of the unit cell and also to state where the atoms are in the repeating unit cell. This is done by giving the position of the atoms as coordinates (x,y,z). The atomic coordinates are given as fractions of the unit length of the vectors. Thus position (0,0,0) is the origo of the unit cell, while the point (1,0,0) is moved (t 1,0,0), i.e. one cell edge along the aaxis parallel to t 1. An atom in the corner of the unit cell therefore has the coordinates (0,0,0), while an atom on the centre of the aaxis has the coordinates (1/2,0,0). As a principal rule, any given atom can be transferred to one or more atoms, of the same type and with the same surroundings, within the unit cell by symmetry operations. In order to describe all the atoms in the unit cell it is enough to give the coordinates of a certain part of the atoms along with the necessary symmetry operations. Within a unit cell one often find several atoms of the same kind. If the surroundings of these atoms are identical, the atoms are related by symmetry operations (they are crystallographic equivalent atoms). If the surroundings are more or less different, the difference is signified by using different notations for the atoms, e.g. Cu(1) and Cu(2), where the number in brackets is just numbering of the same type of element. In such cases one would say that Cu(1) and Cu(2) are not crystallographic equivalent atoms. 2
3 3 Figure 1. The definition of relations between angles and axes in unit cells. The unit cell is shown as the box on the left. Example 1 (2dimensional unit cell) A number of simple structures, e.g. for metals and alloys, may be derived from close packing of spheres. Here the atoms are thought to be ideal, non compressible spheres of the same size. Before we look at such 3dimensional structures in details, we will take a closer look at how symmetrynotation can be used to describe close packing in 2dimensions. Then we will add different symmetry operations, still looking at the 2 dimensional model of the structure. Consider a 2dimensional close packing of identical spheres. The spheres are placed as close as possible (i.e. with the least possible space between them). This is shown to the left below. Let us now define a 2dimensional unit cell for the pattern of repeating spheres. We choose the centre of sphere A as origo. (You will get the same unit cell with any other choice of origo, but there will be less symmetry around the origo). The direction and length of the translation vectors (cell edges) must first be determined. Let t 1 be the vector from the centre of sphere A to the centre of sphere 4, and let t 2 be the vector form the centre of sphere A to the centre of sphere 2. The unit cell is completed by translating t 2 so that it starts in the centre of sphere 4 and t 1 to start in the centre of sphere 2. The lengths of the vectors t 1 and t 2 are called a and b. It is obvious that a and b (= 2r; the radius of the sphere). The angle between t 1 and t 2 can easily be calculated by looking at the equilateral triangle that is formed by the centres of three adjacent spheres. The unit cell is therefore defined as a = b and the angle γ = 120 (look above to the right) This 2dimensional packing of spheres is the closest possible, and such layers constitutes the 2dimensional units that are stacked when making 3dimensional close packed structures (notation AB... = hcp, ABC... = ccp, or more unusual and
4 complicated stacking sequence as e.g. ABAC... An... AA...stacking will not be close packed in 3dimensions even though it is built from 2dimensional close packed units). The values of the coordinates (x, y, z) of a point within the unit cell are all between 0 and 1 (look above). Because the unit cell is a repeating unit, any multipla of the unit vectors can be added to or subtracted from any point (x, y, z), in order to get to identical points in other unit cells. The point (x, y, z) or an atom positioned in A in figure 2, e.g. with coordinates (0.21, 0.33, 0.45) is therefore identical to the point B with the coordinates (0.21, 0.33, 1.45) through the translation (x, y, z+1); and C (0.79, 0.33, 0.45) through the translation (x1, y, z); and D (0.79, 1.33, 0.55) through the translation (x1, y+1, z1). A, B, C and D will have identical surroundings in the unit cell and in any given atomic arrangement in a solid material. When atoms are called identical (equivalent) it means that they have absolute identical surroundings in relation to all nearby points/atoms. In example 1, it is seen that the surroundings of e.g. sphere A and sphere 2 are identical. This means that the spheres with centre at the coordinates (0, 0) and (0, 1) are identical. In reality one can view the two spheres as one and the same. Sphere 2 is just sphere A translated one unit translation (the cell edge) along t 2. All the spheres in example 1 are therefore equivalent, and the 2dimensional packing is completely defined by giving a, b and γ together with the information that there is a sphere in origo. Because the unit cell is a repeating unit, a description of the symmetry and the atom coordinates is the unit cell, will describe the symmetry and structure of the solid material. This is of course only true for crystalline phases, where, as mentioned, a systematic longrange order exists. In amorphous materials there are not repeating unit cells. 4 Figure 2: Same point in several unit cells. The chemical composition of a solid material is given by the ratios between the different kind of atoms in the unit cell. If the unit cell is known, it must be possible to make a correct account of the content. One must take in to consideration that one unit is close up against other unit cells and that it shares faces, edges and corners with the surrounding unit cells. Thus, an atom in a unit cell count as 1, whereas an atom on a face counts as ½ (but this is
5 repeated on the opposite unit cell, and together the two half atoms counts as 1); while an atom in a corner counts as 1/8 (but eight corners share a point, so that 8 1/8 = 1); figure 3. As an illustrated, look at Figure 3 where 8 filled symbols are drawn, two open and one hatched. There are the same number of filled, open and hatched symbols in the repeating unit (one of each). 5 Figure 3. Atoms are placed inside the unit cell (hatched), on the faces (open) and at the corners (filled). The unit cells share faces. Exercise 1 Draw a 2dimensional orthogonal unit cell with cell edges a = 3.80 Å and b = 3.90 Å. Place these atoms in the unit cell: Cu(1) in (0, 0) O(1) in (0, 0.5) O(2) in (0.5, 0) Calculate the distance between Cu and O and between Cu and Cu. Check the calculation against what you would expect based on ion/covalent bonding between cupper and oxygen. Such an atomic arrangement is found in 2dimensional sections of high temperature superconductors. Example 2 (3dimensional unit cell; modes of illustration) Imagine taking the 2dimensional layer of spheres as shown in example 1 and putting it right above the exact same layer. The spheres are positioned right on top of one another, and do not fall down the hollows in the layers. It is obvious that this is not a good utilization of the available volume and that the structure is not close packed in 3 dimensions. Stacking of layers is thought continued in such a way that a 3dimensionel object is built. The unit cell of the 2dimensional layer is exactly as seen in example 1. The repeating length in the stacking direction is given by the vector (t 3 ) from the centre of sphere A to sphere A in the next stacking layer. This vector is perpendicular to t 1 and
6 t 2 in the basal plane. The 3dimensional unit cell is therefore a = b c, α= β = 90 and γ = 120. The unit cell can be drawn like this: 6 The structure that arises from such a stacking is said to be a simple hexagonal packing of the type...aa... (NB not a close hexagonal packing). By using the rules for adding up the spheres/atoms will in a unit cell, one finds that the number of atoms is 8 1/8 = 1, i.e. the unit cell contains a formula unit of spheres/atoms; this is given as Z = 1. Note that when one using the notation packing of spheres and looking at rigid touching spheres, this is of course a model, which does not directly describe the properties of the atoms. Atoms (e.g. the noble gases), ions (e.g. Na +, or Cl  ) and metal atoms (e.g. Fe in metallic iron or a iron containing alloy with metallic conductivity) can to a certain degree be seen as spherical. When we draw a crystal structure, where the spheres of the packing model is replaced by atoms, for clarity they are usually drawn so small, that they do not touch one another (look at the figure above). This is done in order to make the figure easier to interpret. When illustrating how much inner volume there is in e.g. a channel in the structure (e.g. a zeolite) the atoms are drawn with a size proportional to covalent, ionic or Van der Waals radius. It is desirable to describe an actual crystal structure with the highest possible symmetry of the structure. For a given structure, it is quite easy to find several unit cells that all fulfil the criteria of repeatability. The crystallographic unit cell must in addition fulfil other criteria. It must:  Display the maximal symmetry of the structure and  At the same time be the smallest repeating unit that does this *In physics (e.g. in theoretical band structure calculations) an other unit cell, the WignerSeitz cell, is often used. This is the smallest repeating unit, but does not show full translational symmetry. When this is used, it is in order to reduce the complexity by including the smallest possible number of atoms. The crystallographic unit cells may contain many formula units, Z (Z is of course an integer, and takes the value of 2 n 3 m, e.g. 1, 2, 3, 6, etc). The WignerSeitz cell is the smallest repeating closed volume around origo (a lattice point). It contains only one lattice point (see space/bravais lattice) and shows the full rotational symmetry of the crystal system (see below). The WignerSeitz cell is constructed by drawing connecting lines from one lattice point to every neighbouring lattice point. Then perpendicular planes are constructed halfway between the lattice points and the surrounded volume that is defined by the planes is the WignerSeitz cell. This volume can have many faces.*
7 Exercise 2: Estimate which of the four following 2dimensional cells fulfil the requirements of a unit cell. 7 E x e r c i s e 3: Draw the NiAs type structure based exclusively on the basis of the following information: a = b = 3.60 Å, c = 5.10 Å, α = β = 90, γ = 120. Ni(1) in ( 0, 0, 0) Ni(2) in ( 0, 0, 0.5) As(1) in ( ⅓, ⅔, ¼) As(2) in ( ⅔, ⅓, ¾) Draw sketches showing the structure seen slightly from the side and as a projection on the abplane. How many formula units (Z) of NiAs are there per unit cell? SI rules say that pm or nm should be used (in stead of Å) to give the unit cell dimensions. What is the unit cell dimensions of NiAs expressed in pm and nm? Calculate the volume of the unit cell and the volume per formula unit. The density of a material is often determined pycnometrically. This returns a measure of the macroscopic density. Porosity (voids, pores between grains/crystallites) and contaminants will contribute to the measured density being smaller than the theoretical value for the material if it was perfect and built in three dimensions from the atomic arrangement found in the unit cell. Using Xray diffraction it is possible to obtain information about the unit cell dimensions. The socalled Xray density is the density calculated from the crystallographic data for the unit cell, i.e. for a perfect material: ρ = m/v = Z FW/V/N A Where FW is the formula weight, N A is Avogadro s number, V is the unit cell volume and Z is the number of formula units in the unit cell. In a number of materials vacancies are found on crystallographic sites, which would be occupied in a perfect case. In other cases additional atoms are situated on nonframework
8 positions (interstitial atoms). From accurate experimental density data it may be possible to estimate the likely defect structure in strongly defect materials (as e.g. defectgenerating solid solution phases, see Chapter 10 in West) if the density for different defect models can be calculated. Crystal systems Exercise 4. Calculate the Xray density of NiAs. Use data for exercise 3. Would you expect the pycnometrically determined density to be larger or smaller than this? NiAs type phases often have significant nonstoichiometry, i.e. the phases may exist with a small or large compositional region. NiAs does not display nonstoichiometry to any significant extent, but let us assume that the phase has interstitial Niatoms, and can be prepared with a composition Ni 1.01 As. In addition let us assume that the unit cell parameters do not change (which they in practice would). Calculate the Xray density for Ni 1.01 As and compare it with the value calculated for NiAs. There are seven different crystal systems. They differ by having different relations between unit cell axes and angles. The relations between the length of the unit cell axes and the angles between them are given in Table 1 and simple unit cells (with one atom in each corner) are shown in Figure 4. (The notation P in Figure 4 indicate that the unit cells are primitive, i.e. they contain only one point or atom, see section on space lattice). 8 Table 1 Relations Crystal system (t1, t2, t3) a = b = c α = β = γ = 90º Cubic a = b c α = β = γ = 90º Tetragonal a b c α = β = γ = 90º Orthorhombic a b c α = γ; β 90º Monoclinic a b c α β γ 90º Triclinic a = b = c α = β = γ 90º Trigonal (Rhombohedral) a = b c α = β; γ = 120º Hexagonal Figure 4. Schematic representation of the unit cells for the seven crystal systems (drawn with one atom in each corner of the unit cell).
9 9 Exercise 5. Give the formula for the volume of (a) a tetragonal, (b) a monoclinic and (c) a hexagonal unit cell expressed by a, b, c, α, β and/or γ. Crystal systems are arranged hierarchically in such a way that the higher crystal system contains at least one symmetry element that the lower system does not contain, see Figure 5. The cubic system is said to have the highest symmetry, and the triclinic the lowest. The symmetry may be seen as increasing from triclinic, via monoclinic, orthorhombic, hexagonal, tetragonal or rhombohedral to the cubic system. Different crystallographic point groups belong to each of the seven different crystal systems (see below). The crystal systems are characterized by having certain symmetry operations. This is further detailed in the section on crystallographic point groups. Figure 5. Hierarchy of crystal systems. The simplest structure types (atomic arrangements) are metals and disordered alloys that crystallize with one of the close packed atomic arrangements, i.e. hexagonal (hcp, hexagonal close packing) or cubic (ccp, cubic close packing. NB! ccp is equivalent to fcc, face centred cubic). As examples could be mentioned that Mg, subgroup III (group 3) (Sc, Y, La) and subgroup IV (group 4) (Ti, Zr, Hf) have hcp structures, while Ni, Pd, Pt, Cu, Ag and Au have ccp structures. Co has both hcp and ccp phases. Hcp phases belong to the hexagonal crystal system, and ccp to the cubic. The simplest anioncation (metal nonmetal) phases mentioned in West s book are based on close packing of anions with the cations in the small holes. For instance the NaCl, CaF 2 , CsCl and zinc blende structure types belong to the cubic crystal system, NiAstype to the hexagonal crystal system, while rutile belong to the tetragonal crystal system. This means that when unit cell dimensions are tabulated for e.g. NaCl, it is sufficient to give the length of the aaxis, as the other relations (a = b = c, angles = 90º) are given by the cubic symmetry. For TiO 2 with the rutile structure, only the a and caxes are given. Example 3 (Assignment of unit cells) Consider the simple hexagonal unit cell, which was described in example 2. From the axes/anglerelations it is seen to satisfy the conditions for a hexagonal unit cell. Therefore the symmetry is said to be hexagonal. In much the same way a simple primitive cubic unit cell may be described by: a = b = c and α = β = γ = 90º. The unit cell is shown below. The cubic unit cell (looking like a cube) has one atom in each corner. It is sufficient to specify that the unit cell is cubic and to give the length of the aaxis. When the structure is drawn as a projection on the ab plane with the radius of the atoms r = a/2, the atoms will touch, and it will be evident that the structure is not close packed, as there are big voids between the spheres.
10 10 Example 4. (Close packing of spheres in three dimensions) Again the starting point is the twodimensional packing of spheres from example 1. Such a layer is close packed. Closer consideration reveals that the spheres touch and are placed like pearls on a string in three directions. Thus, in a close packed layer of spheres there are three close packed directions. If such layers are stacked on top of each other (along the caxis) and systematically shifted with respect to each other in such a way that the spheres of one layer is positioned above the holes of the layer below, a three dimensional close packing of spheres is obtained. This may be best illustrated by drawing the layers on individual transparent foils: Consider one layer. On this layer you draw the twodimensional unit cell described in example 1. The centre of atom A is the origo of the twodimensional unit cell. We now choose this position as the origin of the threedimensional unit cell, which we will derive from stacking of several close packed layers. The Asphere therefore has the position (coordinate) (0,0,0). Also the spheres numbered 2, 3, and 4 in example 1 are described with this position. This is because their positions may be generated by adding to the position (0, 0, 0) multipla of the twodimensional unit cell translations. This means that the position of all the spheres in the layer, which we now will call layer A, are given as (0+n, 0+m, 0) where n and m are integers. Consider the four spheres in the unit cell. Between the spheres there are two indentations, between the 3 spheres A, 4 and 3, and between A, 2 and 3, respectively. We may call the positions which characterize the two indentations B and C. Consider now e.g. the triangle A,4,3 and the point B. By a bit of trigonometry the coordinates (2/3, 1/3) is found for B and (1/3, 2/3) for C. We define two new 2dimentional sheets, named B and C, identical to the A sheet. The B sheet is placed so that there is a sphere right above the B position in the A sheet. The spheres of the B sheet have the coordinates (2/3, 1/3) relative to the chosen origo of the A sheet. In the same way the C sheet is placed so that the spheres have the coordinates (1/3, 2/3) relative to the chosen origo of sheet A. By adding layers on top of each other and using the indentations one obtains a 3dimensional close packing. If the repeating sequence of layer positions is...ab..., it is a hexagonal closest packing (hcp), if the sequence is...abc... it is a cubic close packing (ccp).
11 Any (more complicated) ordering of layers is also a close packing, if there are no layers directly above an identical layer (i.e. there is no...aa...,...bb... or...cc... sequence). The simple ordering sequences are those mentioned above,...ab... and...abc... However in many cases there is very little difference in energy between different ordering sequences for real materials, and the material has many different modifications. The ordering sequences may be complicated (e.g....abcacbcab...). The different ordering variants are called polytypes. These have an identical structure in twodimentions, but some differences in the third dimension, the ordering direction. Polytypes are known in compounds such as Co, SiC, ZnS, ABO 3 and others. 11 schematic ordered stacking of sheets seen from the side (not 100 % correct displacement along the side) Space lattice. The notation space lattice or lattice (romgitter) is a mathematical description of repeating units in solid materials. It is important to realize that a lattice is not the same as a structure. A structure is the atomic arrangement, whereas a lattice is made of mathematical points in space, and these may be translated by certain operations. The similarity between a lattice and the unit cell is striking, especially for the primitive space lattices. The primitive space lattices contain only one point in the repeating unit, and it is placed in the corners of the unit. The different repeating units were described in Unit cells and Crystal systems. There are 7 possibilities, and so there are 7 primitive space lattices. The relations between the translation vectors are also described above. Figure 4 was used to illustrate simple unit cells. The drawings in figure 4 may also represent the primitive space lattices with a lattice point placed in each corner. The primitive lattices are denoted with a P. The primitive rhombohedral is an exception to this rule it is denoted with R. Example 5 (primitive space lattices): Consider the primitive hexagonal space lattice. A (lattice)point (x, y, z) is transferred to equivalent points in the lattice by the translation vectors (t 1, t 2, t 3 ). New (lattice)points have the coordinates (x+nt 1,y+mt 2, z+ot 3 ), where n, m and o are integers. This is drawn in a 2dimentionel projection below. Consider the objects below. They are meant to represent a fragment of a structure. We see that the fragment is repeated in two dimensions. The repetition may be described as (new fragment) = (original fragment) + lattice translation. We choose a random point in one of the fragments, and mark similar points in the other fragments. These
12 points can now be connected by translation vectors t 1 and t 2, which are translation vectors of the 2dimentional, primitive lattice. 12 An absolute requirement to a space lattice is identical surroundings around every single lattice point. This is the starting point to the consideration whether there can be other space lattices than the primitive space lattices described above. It turns out, that all in all there are 14 different lattices which met the requirement. They are called Bravais lattices and are described below. Bravais lattices. It is relatively easy to prove that there are a total of 14 threedimensional lattices which met the criteria of identical surroundings of the lattice points. These are called Bravais lattices, see figure 6. Seven of these are the primitive lattices described above. Figure 6. The 14 Bravais lattices. The primitive Bravais lattices contain only one lattice point. The non primitive Bravais lattices contain more than one lattice point per unit cell (2 or 4), and are called centred lattices:
13 Bodycentred lattice (notation I for Innenzentrierung, new lattice point in a/2 + b/2 + c/2) Facecentred lattice (F, Flächenzentrierung, new lattice points a/2 + b/2 and + a/2 + c/2 and b/2 + c/2) Sidecentred lattice (A, B or C, side centred on only some of the sides, e.g. a/2 + b/2. This is a C side centred lattice, which means that the centring are on the sides normal to the c direction/z axes) The four different types of lattices are illustrated by the orthorhombic Bravais lattices in figure 6. The Bravais lattices matching the crystal systems are given in table 2. Example 6 (Bravais lattices) Close packed, hcp and ccp, have a primitive hexagonal Bravais lattice and a face centred cubic Bravais lattice, respectively (see example 7). The relationship between the ccp packing and the cubic unit cell is discussed in West (see figure 7.5) but the relationship may be somewhat difficult to see. The close packed layers in the ccp structure lies perpendicular to the space diagonals in the cubic cell. The cubic unit cell has atoms placed in the corners and in the center of all the faces. If we neglect that there are atoms in the cell and replace them with mathematical points, it is clear that it is a cubic Bravais lattice with F centring. If an atom is placed at every lattice point, the face centred cubic structure is reached. This is known as fcc. This is also identical to ccp. For a fccmetal Z = 4. Table 2: Crystal system Bravais lattice Z Cubic P 1 I 2 F 4 Tetragonal P 1 I 2 Orthorhombic P 1 I 2 C 2 F 4 Monoclinic P 1 C 2 Triclinic P 1 Rombohedral R 1 Hexagonal P 1 The centred Bravais lattices may also be represented by smaller primitive unit cells. These will however not show the highest symmetry of the system, which is a requirement for a crystallographic unit cell. See figure 7. Exercise 6: Show how the cubic FBravais lattice fulfils the requirements of a lattice (consider the surroundings of every lattice point). 13
14 Exercise 7: Draw a tetragonal P lattice. Place an extra lattice point in ½, ½, 0, i.e. make a C centring of the lattice. Show that a tetragonal C lattice does not exist as such, i.e., that it is equivalent to (another) P lattice. Brasvais lattices define the way a lattice point (ore a fragment of a structure, see example 5) is transferred to identical points (ore fragments). A crystal structure can therefore be described as structure = lattice + basis where the basis is made of the repeating structure fragment with a number of atoms with coordinates (x i, y i, z i ). 14 Figure 7. Relationship between primitive cells and F, I and C centred cells. Some simple crystal structures are shown in Figure 8. From these it is possible to say what type of Bravais lattice the different structure types has. E.g. CsCl type structure has a Bravais lattice Pcubic, NaCl and CaF 2 type have a Fcubic, NiAs type is Phexagonal, whereas bcc (metal) has a Icubic Bravais lattice. How this is seen is explained in example 7. Figure 8. Schematic representation of NaCl, CaF 2 , CsCl and bcc type crystal structure. The symbols below the figures are space group notation. Example 7 (Bravais lattice): In this example we take a closer look at the CsCl type structure and hcp. In CsCl (figure 8) the black spheres form a primitive cubic lattice (a=b=c, angles = 90º). The sphere in the centre is of another type and has nothing to do with the lattice of the black spheres. If several unit cells are drawn beside each other, it is possible to see which repeating rules that can be applied to the open spheres. You will find that the repeating unit is an identical cubic box with the same edge as the one of the black spheres. The Bravais lattice is the same, but because the spheres are different, they both are part of the basis of the structure; i.e. the CsCl type structure has a cubic P lattice with Cs in (0, 0, 0) and Cl in (½, ½, ½). This can be seen as: CsCl type structure = cubic Plattice + basis [Cs in (0, 0, 0) and Cl in ((½, ½, ½)]
15 15 It is also easy to show that the hcp structure has a primitive hexagonal Bravais lattice. Look at the figure below. The open spheres represent sheet A, the black sheet B, as in previous examples. Four unit cells (with a sphere A in origo) are marked with a full line. Consider now the 4 B spheres. They define a unit cell as well (dotted line) which in shape and size is identical to the one defined by the Aspheres. The only difference is that the Bcells origo has been moved to (2/3, 1/3). In order to describe the hcp structure, the Bravais lattice can be said to be hexagonal primitive and basis to be two atoms in respectively (0, 0, 0) and (2/3, 1/3, 1/2); i.e. hcp type structure = hexagonal Plattice + basis [M in (0, 0, 0) and M in (2/3, 1/3, 1/2)] A better description is given in example 9, where symmetry elements are considered as well. Symmetry operations Exercise 8: Draw the structure of the anioncation compound AB on the basis of the following information: The Bravais lattice is Fcubic Basis: A atom in (0, 0, 0) and B atom in (1/2, 0, 0) What is the name of this type of structure? Exercise 9: Ni has a cubic face centred structure, known as fcc, i.e. face centred cubic with basis: Ni in (0, 0, 0). The cell edge is 351 pm. Calculate the radius of the Ni spheres (metallic radius). Calculate the density of Ni. In the following we will consider symmetry operations that can be used to describe isolated objects, e.g. a molecule in gas phase. The requirement of a symmetry operation is that when it operates (is used) on an atom with a set of atomic coordinates (x, y, z), an atom of the same type and with identical surroundings is created, but with the coordinates (x, y, z ). These are the symmetry elements which exist:  Identity, that is (x, y, z) is transferred to itself (x, y, z). This symmetry element is included, because it is a requirement in the definition of a group in group theory, which is the mathematical tool used in symmetry considerations.  Inversion, that is (x, y, z) is translated to (x, y, z). If an object has this symmetry element, it is said to be centrosymmetric (det er sentrosymmetrisk).
16  Rotation axis, a rotation axis is two fold, three fold etc. A nfold axis rotate an object 360º/n.  Mirror plane which places the object laterally reversed (mirror image) as far behind the mirror plane as it was in front. E.g. an xymirror plane (i.e. the xy plane is thought to be the plane of the mirror) transfers a point (x, y, z) to (x, y, z). Inversion symmetry and mirror planes both transfers a right handed object to a left handed object (like a mirror image; this is shown by writing a comma (,) in the circles, as shown in figure 9. The effect of these symmetry operations is schematically shown with hands in figure 9. The nomenclature (symbols) are also shown. 16 Figure 9: Inversion, reflection and two fold axes. The effect of the operations is shown with hands. The use of symbols is further described in point groups. The origin of the symmetry operations and the coordinate system are chosen so as to reveal the highest possible symmetry. Two sets of nomenclature are used to indicate symmetry operations. Schönflies nomenclature is often used in spectroscopy, whereas HermannMauguin nomenclature is used in crystallography (description of structure). The notation is different, but the operations are of course the same, see Table 3. Table 3 Symmetry operation Schönflies symbol HermannMauguin symbol Identity E or I I Inversion i (centro symmetric) Rotation axis C n (n=fold) n Mirror plane σ h, σ v m (reflection) σ h and σ v are the notation for the horizontal and the vertical mirror plane respectively (defined relative to the main rotation axis. Exercise 10: Which symmetry operations can you identify for the following objects: (a) H 2 O (b) NH 3 (c) CO 2 (d) CH 4 (e) a d xy orbital There are also combined symmetry operations, which means that two symmetry operations are performed right after each other and thus the intermediate state is not considered. Rotationinversion axes are used in crystallography [rotationinversion axes are denoted as n, often expressed as n ], i.e. a nfold rotation is done followed by an inversion. In the _ 1
17 Schönflies notation rotationinversion axes are denoted S n. Some examples of such symmetry operations are shown in figure 10. Exercise 11: The tetrahedron belongs to the group of objects with a symmetry in the cubic system. Compare the 4fold rotation axes in a cube and in a tetrehedra. 17 Figure 10: Symmetry operations 4, 6, 4 & 6. Example 8 (Rotation axes, crystal system) Let us consider hcp close packing. Let us first consider a 2dimensional A sheet, and choose origo to be in the centre of a chosen sphere. We can now evaluate the nfold rotation axis perpendicular to the close packed sheet. By a rotation of 60º the picture is identical, i.e. we have a 360º/60º = 6fold rotation axis. This is characteristic for the hexagonal crystal system, cf. Table 5. If we construct an AB packing, we see that the 6fold axes is not preserved, but in each sheet there are points with a 6fold symmetry. This is discussed further in the paragraph on glide planes and screw axes. Example 9 (Choise of origo, center of symmetry): We consider at a projection of the hcp structure onto the ab plane: Let us evaluate if this unit cell has an inversion center, i.e. it is centro symmetric. In this case all atomic coordinates, were given relative to the centre of symmetry placed in origo, must be transferred to identical coordinates for atoms by the inversion operation (x i, y i, z i ) (x i, y i, z i ) If the origin chosen at the centre of an Aatom (open symbol, solid unit cell) we see that there are no centro symmetric surrounding A. For atom B with coordinates (2/3, 1/3, 1/2) there are no identical B or Aatoms (A and B are identical atoms/spheres)
18 with coordinates (1/3, 2/3, 1/2) = (2/3, 1/3, 1/2) = (2/3 +1, 1/3 +1, 1/2+1); see solid arrow. The apparent lack of centro symmetry is actually due to the fact that we have chosen the wrong point as the centre of symmetry. Let us choose the point (1/3, 2/3, 1/4) as origo, which is assumed to be a centre of symmetry. First the coordinates in sheet A and B must be transformed to (01/3, 02/3, 01/4) = (2/3, 1/3, 3/4) and (2/3 1/3, 1/3 2/3, 1/2 1/4) = (1/3, 2/3, 1/4), respectively. It is now easy to see that a centre of symmetry relates sheet A and sheet B, cf. the dotted arrow. The hcp structure is therefore centro symmetric. The unit cell with a center of symmetry in origo is dotted. A closer look at the figure reveals that there are more points, which are center of symmetry than (0, 0, 0). 18 Point groups. A point group is described by a characteristic assembly of symmetry operations. A certain number of symmetry operations with defined geometrical relations among themselves can be found for any given object. The object is said to have symmetry described by the given point group. Different objects which have different symmetry will therefore be described with different point groups. All symmetry elements present refer to a common point, the origo. *A point group must fulfil the mathematical requirements of a group:  The product of two operations is another operation in the group  The identity element (I) is present  The existence of an inverse operator RR 1 = 1  Associative multiplication of operations* The point groups have different notation in Schönflies and HermannMauguin nomenclature. In Schönflies nomenclature there are point groups such as C nv, C nh, D nh, T d, O h etc, where n is the highest number of rotation axes present and v is the vertical mirror plane, which is only mentioned if there are no horizontal mirror planes (h). If there are twofold axes perpendicular to the highest rotation axes, the point group is D nh. T is a tetrahedral and O is an octahedral point group (cubic crystal system). In the HermannMauguin nomenclature similar information is given. The highest rotation axis is given first. E.g. a point group with only a twofold rotation axes is denotated 2. C 2h (Schönflies) is notated 2/m, where the slash indicate that the mirror plane is perpendicular to the twofold axis. In the following only the HermannMauguin nomenclature is used. The two types of nomenclature are compared for a number of point groups in Table 4. Table 4. HermannMauguin nomenclature: /m 3 4/m 6/m mmm 3 m 4/mmm 6/mmm m3 m3m Schönflies nomenclature: C 1 C 2 C 3 C 4 C 6 D 2 D 3 D 4 D 6 T O C i C 2h S 6 C 4h C 6h D 2h D 3d D 4h D 6h T h O h
19 19 Example 10 (point symmetry): Consider a small section of the close packing in twomensions in example 1 by choosing one sphere and the surrounding six. First we define the directions by letting the a and baxes be in the basal plane as shown in example 1. We let the caxis be perpendicular to the abplane. The relations between the axes are those required in the hexagonal crystal system. We observe a 6fold rotation axis runs through the central sphere and parallel to the caxis. The basal plane is a mirror plane. Therefore the HermannMauguin symbol must be 6/m. The full symbol is larger because all information on the symmetry relations along the axes in the basal plane must be given as well. This is described in the second part of the example below. Exercise 12. Give the Schönflies and HermannMauguin symbols for point groups with the following symmetry elements: (a) a fourfold rotation axis (b) identity and an inversion axis (c) a fourfold rotation axis and a mirror plane perpendicular to the rotation axis. Exercise 13: Which symmetry elements can you identify in the point groups: (a) 1 (b) 3 (c) 6/m (d) 4/m For isolated objects there is no limit on the n fold of a rotation axis. Therefore one can imagine an infinite number of point groups, but only a few of these are found frequently in real objects. A fivefold rotation axis exists e.g. in an isolated flat C 5 H 5 molecule. Global fivefold symmetry cannot appear in ordered, threedimensional crystalline phases. On the other hand it is possible to observe units with a local fivefold symmetry in solid materials, even though it is not possible to fit 5fold symmetry into a repeating lattice (see below). The point group symbol tells which symmetry elements are essential to the point group (these may create other symmetry elements by being used on each other). Consider e.g. the point group 2/m. The symbol reveals that there is a twofold rotation axis and a horizontal mirror plane. Because these elements are both present, the inversion element is automatically present too, figure 11. Thus, 2/m is a centro symmetrical point group. All in all the point group 2/m contain the symmetry operations. Identity, twofold rotation axis, horizontal mirror plane and inversion. Figure 11. Structure fragment with point symmetry 2/m.
20 20 Those point groups which contain an inversion element are considered centro symmetrical. Certain properties in a material depend on the symmetry, e.g. the existence of electric dipoles, optic activity, pyro and piezoelectricity. The last two are discussed in chapter 15 in West (not part of the curriculum). Exercise 14: Explain why a molecule with a permanent electric dipole (i.e. the molecule has a dipole moment) cannot be centro symmetric. Can a material built by hcppacking display permanent polarization (i.e. have a total sum of dipole moments that is not zero)? So far we have limited the description to cases with one rotation axis and one mirror plane (vertical or horizontal). If the description is extended to include also symmetry relations in orthogonal directions, the result is a number of new point groups. One can e.g. imagine a point group with three twofold rotation axes, in the directions x, y and z in a cartesian coordinate system. This point group is called 222 (orthorhombic system) where all the symbols (the 2 s) describe the symmetry relations in the orthogonal directions. The combined point group symbols e.g. mm2 are interpreted following certain rules. For example the first symbol for orthorhombic and tetragonal point groups describes the symmetry along the zaxis (which is thereby chosen to have the highest rotation axis in the tetragonal crystal system), the next symbol describes the relations in a perpendicular direction (e.g. the yaxis) and in the orthorhombic system the last symbol describes the relations in the third direction, whereas in the tetragonal system it describes the symmetry in the [110] direction. More specialized rules for symbol, 2 and 3 must be used for trigonal, hexagonal and cubic point groups. Example 10 (point symmetry, continued): In the hexagonal crystal system the first part of the combined point group symbol describes the symmetry conditions along the caxis, the next the conditions along the a and baxes, and the third the conditions along a direction perpendicular to the a and baxes. If we look at the isolated object (1+6 spheres) we see that the aaxis is a twofold rotation axis with a perpendicular mirror plane, i.e. with the symbol 2/m. We also note that perpendicular to the aaxis there is another twofold rotation axis with a perpendicular mirror plane. The correct point group symbol is therefore 6/m2/m2/m. Exercise 15: Consider the flat molecule transdichloroethen C 2 H 2 Cl 2. Draw the molecule in the xyplane (let the zdirection be the direction with the twofold axis). Identify the symmetry operations I, C 2 z, σ h xy and i (in Schönflies nomenclature). What are these called in HermannMauguin nomenclature? Explain why the point group symbol is C 2h (Schönflies). How would you describe the point group with crystallographic nomenclature? Show that the assembly of symmetry elements fulfils the requirements of a group. The point groups are classified under the different crystal systems. For a given crystal system certain characteristic symmetry elements can be identified, see Table 5. Note that the cubic crystal system is not characterized by the presence of fourfold axes, but by the existence of four threefold axes.
Solid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationEarth Sciences: Course Presenters
Earth Sciences: Course Presenters 625102 Geology Dr Stephen Gallagher Prof Andrew Gleadow Dr Malcolm Wallace Prof Ian Plimer Course Coordinator Room 214 Series  Lecture Topics 1. Mineralogy and Crystals
More informationCoordination and Pauling's Rules
Page 1 of 8 EENS 2110 Tulane University Mineralogy Prof. Stephen A. Nelson Coordination and Pauling's Rules This document last updated on 24Sep2013 The arrangement of atoms in a crystal structure not
More informationCrystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationChapter 2: Crystal Structures and Symmetry
Chapter 2: Crystal Structures and Symmetry Laue, ravais December 28, 2001 Contents 1 Lattice Types and Symmetry 3 1.1 TwoDimensional Lattices................. 3 1.2 ThreeDimensional Lattices................
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationNumber Sense and Operations
Number Sense and Operations representing as they: 6.N.1 6.N.2 6.N.3 6.N.4 6.N.5 6.N.6 6.N.7 6.N.8 6.N.9 6.N.10 6.N.11 6.N.12 6.N.13. 6.N.14 6.N.15 Demonstrate an understanding of positive integer exponents
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More information11.1. Objectives. Component Form of a Vector. Component Form of a Vector. Component Form of a Vector. Vectors and the Geometry of Space
11 Vectors and the Geometry of Space 11.1 Vectors in the Plane Copyright Cengage Learning. All rights reserved. Copyright Cengage Learning. All rights reserved. 2 Objectives! Write the component form of
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationTwo vectors are equal if they have the same length and direction. They do not
Vectors define vectors Some physical quantities, such as temperature, length, and mass, can be specified by a single number called a scalar. Other physical quantities, such as force and velocity, must
More informationMatter, Materials, Crystal Structure and Bonding. Chris J. Pickard
Matter, Materials, Crystal Structure and Bonding Chris J. Pickard Why should a theorist care? Where the atoms are determines what they do Where the atoms can be determines what we can do Overview of Structure
More informationChapter 13  LIQUIDS AND SOLIDS
Chapter 13  LIQUIDS AND SOLIDS Problems to try at end of chapter: Answers in Appendix I: 1,3,5,7b,9b,15,17,23,25,29,31,33,45,49,51,53,61 13.1 Properties of Liquids 1. Liquids take the shape of their container,
More informationAdding vectors We can do arithmetic with vectors. We ll start with vector addition and related operations. Suppose you have two vectors
1 Chapter 13. VECTORS IN THREE DIMENSIONAL SPACE Let s begin with some names and notation for things: R is the set (collection) of real numbers. We write x R to mean that x is a real number. A real number
More informationElectroceramics Prof. Ashish Garg Department of Material Science and Engineering Indian Institute of Technology, Kanpur.
Electroceramics Prof. Ashish Garg Department of Material Science and Engineering Indian Institute of Technology, Kanpur Lecture  3 Okay, so in this third lecture we will just review the last lecture,
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationCHAPTER 10: INTERMOLECULAR FORCES: THE UNIQUENESS OF WATER Problems: 10.2, 10.6,10.1510.33, 10.3510.40, 10.5610.60, 10.10110.
CHAPTER 10: INTERMOLECULAR FORCES: THE UNIQUENESS OF WATER Problems: 10.2, 10.6,10.1510.33, 10.3510.40, 10.5610.60, 10.10110.102 10.1 INTERACTIONS BETWEEN IONS Ionion Interactions and Lattice Energy
More informationAP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts
AP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts 8.1 Types of Chemical Bonds A. Ionic Bonding 1. Electrons are transferred 2. Metals react with nonmetals 3. Ions paired have lower energy
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More informationSolid Type of solid Type of particle
QUESTION (2015:3) Complete the table below by stating the type of solid, the type of particle, and the attractive forces between the particles in each solid. Solid Type of solid Type of particle Cu(s)
More informationPart 432 point groups
Part 432 point groups 4.1 Subgroups 4.2 32 point groups 4.2 Crystal forms The 32 point groups The point groups are made up from point symmetry operations and their combinations. A point group is defined
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationThe Structure of solids.
Chapter S. The Structure of solids. After having studied this chapter, the student will be able to: 1. Distinguish between a crystal structure and an amorphous structure. 2. Describe the concept of a unit
More informationLaboratory 11: Molecular Compounds and Lewis Structures
Introduction Laboratory 11: Molecular Compounds and Lewis Structures Molecular compounds are formed by sharing electrons between nonmetal atoms. A useful theory for understanding the formation of molecular
More informationDIRECTEDDISCOVERY OF CRYSTAL STRUCTURES USING BALL AND STICK MODELS
DIRECTEDDISCOVERY OF CRYSTAL STRUCTURES USING BALL AND STICK MODELS David W. Mogk Dept. of Earth Sciences Montana State University Bozeman, MT 59717 dmogk@montana.campus.mci.net INTRODUCTION Understanding
More informationA pure covalent bond is an equal sharing of shared electron pair(s) in a bond. A polar covalent bond is an unequal sharing.
CHAPTER EIGHT BNDING: GENERAL CNCEPT or Review 1. Electronegativity is the ability of an atom in a molecule to attract electrons to itself. Electronegativity is a bonding term. Electron affinity is the
More informationrotation,, axis of rotoinversion,, center of symmetry, and mirror planes can be
Crystal Symmetry The external shape of a crystal reflects the presence or absence of translationfree symmetry y elements in its unit cell. While not always immediately obvious, in most well formed crystal
More informationFURTHER VECTORS (MEI)
Mathematics Revision Guides Further Vectors (MEI) (column notation) Page of MK HOME TUITION Mathematics Revision Guides Level: AS / A Level  MEI OCR MEI: C FURTHER VECTORS (MEI) Version : Date: 97 Mathematics
More information121 Representations of ThreeDimensional Figures
Connect the dots on the isometric dot paper to represent the edges of the solid. Shade the tops of 121 Representations of ThreeDimensional Figures Use isometric dot paper to sketch each prism. 1. triangular
More informationEXPERIMENT 9 Dot Structures and Geometries of Molecules
EXPERIMENT 9 Dot Structures and Geometries of Molecules INTRODUCTION Lewis dot structures are our first tier in drawing molecules and representing bonds between the atoms. The method was first published
More informationChapter 11. Chemical Bonds: The Formation of Compounds from Atoms
Chapter 11 Chemical Bonds: The Formation of Compounds from Atoms 1 11.1 Periodic Trends in atomic properties 11.1 Periodic Trends in atomic properties design of periodic table is based on observing properties
More informationCurrent Standard: Mathematical Concepts and Applications Shape, Space, and Measurement Primary
Shape, Space, and Measurement Primary A student shall apply concepts of shape, space, and measurement to solve problems involving two and threedimensional shapes by demonstrating an understanding of:
More informationCHAPTER NOTES CHAPTER 16. Covalent Bonding
CHAPTER NOTES CHAPTER 16 Covalent Bonding Goals : To gain an understanding of : NOTES: 1. Valence electron and electron dot notation. 2. Stable electron configurations. 3. Covalent bonding. 4. Polarity
More informationBiggar High School Mathematics Department. National 5 Learning Intentions & Success Criteria: Assessing My Progress
Biggar High School Mathematics Department National 5 Learning Intentions & Success Criteria: Assessing My Progress Expressions & Formulae Topic Learning Intention Success Criteria I understand this Approximation
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationNuclear reactions determine element abundance. Is the earth homogeneous though? Is the solar system?? Is the universe???
Nuclear reactions determine element abundance Is the earth homogeneous though? Is the solar system?? Is the universe??? Earth = anion balls with cations in the spaces View of the earth as a system of anions
More informationCommon Core Unit Summary Grades 6 to 8
Common Core Unit Summary Grades 6 to 8 Grade 8: Unit 1: Congruence and Similarity 8G18G5 rotations reflections and translations,( RRT=congruence) understand congruence of 2 d figures after RRT Dilations
More informationKEANSBURG SCHOOL DISTRICT KEANSBURG HIGH SCHOOL Mathematics Department. HSPA 10 Curriculum. September 2007
KEANSBURG HIGH SCHOOL Mathematics Department HSPA 10 Curriculum September 2007 Written by: Karen Egan Mathematics Supervisor: Ann Gagliardi 7 days Sample and Display Data (Chapter 1 pp. 447) Surveys and
More informationCapacitance and Ferroelectrics
Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity
More informationSymmetry and group theory
Symmetry and group theory or How to Describe the Shape of a Molecule with two or three letters Natural symmetry in plants Symmetry in animals 1 Symmetry in the human body The platonic solids Symmetry in
More informationFigure 1.1 Vector A and Vector F
CHAPTER I VECTOR QUANTITIES Quantities are anything which can be measured, and stated with number. Quantities in physics are divided into two types; scalar and vector quantities. Scalar quantities have
More informationCrystalline Structures Crystal Lattice Structures
Jewelry Home Page Crystalline Structures Crystal Lattice Structures Crystal Habit Refractive Index Crystal Forms Mohs Scale Mineral Classification Crystal Healing Extensive information on healing crystals,
More informationDO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS
DO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS Quantum Mechanics or wave mechanics is the best mathematical theory used today to describe and predict the behaviour of particles and waves.
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More information2C Intermolecular forces, structure and properties:
Electronegativity and polarity Polar and nonpolar bonds: 1) NonPolar bonds: 2C Intermolecular forces, structure and properties: A covalent bond shares an electron pair: In a hydrogen molecule, the electrons
More informationPOLAR COVALENT BONDS Ionic compounds form repeating. Covalent compounds form distinct. Consider adding to NaCl(s) vs. H 2 O(s):
POLAR COVALENT BONDS Ionic compounds form repeating. Covalent compounds form distinct. Consider adding to NaCl(s) vs. H 2 O(s): Sometimes when atoms of two different elements form a bond by sharing an
More informationNEW MEXICO Grade 6 MATHEMATICS STANDARDS
PROCESS STANDARDS To help New Mexico students achieve the Content Standards enumerated below, teachers are encouraged to base instruction on the following Process Standards: Problem Solving Build new mathematical
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationMATHS LEVEL DESCRIPTORS
MATHS LEVEL DESCRIPTORS Number Level 3 Understand the place value of numbers up to thousands. Order numbers up to 9999. Round numbers to the nearest 10 or 100. Understand the number line below zero, and
More informationCHAPTER 6 Chemical Bonding
CHAPTER 6 Chemical Bonding SECTION 1 Introduction to Chemical Bonding OBJECTIVES 1. Define Chemical bond. 2. Explain why most atoms form chemical bonds. 3. Describe ionic and covalent bonding.. 4. Explain
More information6. Vectors. 1 20092016 Scott Surgent (surgent@asu.edu)
6. Vectors For purposes of applications in calculus and physics, a vector has both a direction and a magnitude (length), and is usually represented as an arrow. The start of the arrow is the vector s foot,
More informationChapter 4: Structure and Properties of Ionic and Covalent Compounds
Chapter 4: Structure and Properties of Ionic and Covalent Compounds 4.1 Chemical Bonding o Chemical Bond  the force of attraction between any two atoms in a compound. o Interactions involving valence
More informationKINETIC MOLECULAR THEORY OF MATTER
KINETIC MOLECULAR THEORY OF MATTER The kineticmolecular theory is based on the idea that particles of matter are always in motion. The theory can be used to explain the properties of solids, liquids,
More informationAlgebra 1 2008. Academic Content Standards Grade Eight and Grade Nine Ohio. Grade Eight. Number, Number Sense and Operations Standard
Academic Content Standards Grade Eight and Grade Nine Ohio Algebra 1 2008 Grade Eight STANDARDS Number, Number Sense and Operations Standard Number and Number Systems 1. Use scientific notation to express
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationUnderstand the Sketcher workbench of CATIA V5.
Chapter 1 Drawing Sketches in Learning Objectives the Sketcher WorkbenchI After completing this chapter you will be able to: Understand the Sketcher workbench of CATIA V5. Start a new file in the Part
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationA reinterpretation of the phase transitions in Na 2 CO 3
Acta Crystallographica Section B Structural Science ISSN 01087681 Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International
More informationIonic and Metallic Bonding
Ionic and Metallic Bonding BNDING AND INTERACTINS 71 Ions For students using the Foundation edition, assign problems 1, 3 5, 7 12, 14, 15, 18 20 Essential Understanding Ions form when atoms gain or lose
More informationChapter 22: Electric Flux and Gauss s Law
22.1 ntroduction We have seen in chapter 21 that determining the electric field of a continuous charge distribution can become very complicated for some charge distributions. t would be desirable if we
More informationdiscuss how to describe points, lines and planes in 3 space.
Chapter 2 3 Space: lines and planes In this chapter we discuss how to describe points, lines and planes in 3 space. introduce the language of vectors. discuss various matters concerning the relative position
More information100 Math Facts 6 th Grade
100 Math Facts 6 th Grade Name 1. SUM: What is the answer to an addition problem called? (N. 2.1) 2. DIFFERENCE: What is the answer to a subtraction problem called? (N. 2.1) 3. PRODUCT: What is the answer
More informationAngles that are between parallel lines, but on opposite sides of a transversal.
GLOSSARY Appendix A Appendix A: Glossary Acute Angle An angle that measures less than 90. Acute Triangle Alternate Angles A triangle that has three acute angles. Angles that are between parallel lines,
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationTheme 3: Bonding and Molecular Structure. (Chapter 8)
Theme 3: Bonding and Molecular Structure. (Chapter 8) End of Chapter questions: 5, 7, 9, 12, 15, 18, 23, 27, 28, 32, 33, 39, 43, 46, 67, 77 Chemical reaction valence electrons of atoms rearranged (lost,
More informationChem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry
Chem 115 POGIL Worksheet  Week 4 Moles & Stoichiometry Why? Chemists are concerned with mass relationships in chemical reactions, usually run on a macroscopic scale (grams, kilograms, etc.). To deal with
More information5. Structure, Geometry, and Polarity of Molecules
5. Structure, Geometry, and Polarity of Molecules What you will accomplish in this experiment This experiment will give you an opportunity to draw Lewis structures of covalent compounds, then use those
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationChapter 18 Symmetry. Symmetry of Shapes in a Plane 18.1. then unfold
Chapter 18 Symmetry Symmetry is of interest in many areas, for example, art, design in general, and even the study of molecules. This chapter begins with a look at two types of symmetry of twodimensional
More information100% ionic compounds do not exist but predominantly ionic compounds are formed when metals combine with nonmetals.
2.21 Ionic Bonding 100% ionic compounds do not exist but predominantly ionic compounds are formed when metals combine with nonmetals. Forming ions Metal atoms lose electrons to form +ve ions. Nonmetal
More informationLiquids and Solids. AP Chemistry Chapter 10. 9/20/2009 Jodi Grack; Wayzata High School; images used with permission from Zumdahl
Liquids and Solids AP Chemistry Chapter 10 Liquids and Solids Gases are much easier to study because molecules move independent of each other. In liquids and solids forces between molecules become very
More informationEXPERIMENT 17 : Lewis Dot Structure / VSEPR Theory
EXPERIMENT 17 : Lewis Dot Structure / VSEPR Theory Materials: Molecular Model Kit INTRODUCTION Although it has recently become possible to image molecules and even atoms using a highresolution microscope,
More informationWafer Manufacturing. Reading Assignments: Plummer, Chap 3.1~3.4
Wafer Manufacturing Reading Assignments: Plummer, Chap 3.1~3.4 1 Periodic Table Roman letters give valence of the Elements 2 Why Silicon? First transistor, Shockley, Bardeen, Brattain1947 Made by Germanium
More informationType of Chemical Bonds
Type of Chemical Bonds Covalent bond Polar Covalent bond Ionic bond Hydrogen bond Metallic bond Van der Waals bonds. Covalent Bonds Covalent bond: bond in which one or more pairs of electrons are shared
More information1.7 Cylindrical and Spherical Coordinates
56 CHAPTER 1. VECTORS AND THE GEOMETRY OF SPACE 1.7 Cylindrical and Spherical Coordinates 1.7.1 Review: Polar Coordinates The polar coordinate system is a twodimensional coordinate system in which the
More informationUnified Lecture # 4 Vectors
Fall 2005 Unified Lecture # 4 Vectors These notes were written by J. Peraire as a review of vectors for Dynamics 16.07. They have been adapted for Unified Engineering by R. Radovitzky. References [1] Feynmann,
More informationEVERY DAY COUNTS CALENDAR MATH 2005 correlated to
EVERY DAY COUNTS CALENDAR MATH 2005 correlated to Illinois Mathematics Assessment Framework Grades 35 E D U C A T I O N G R O U P A Houghton Mifflin Company YOUR ILLINOIS GREAT SOURCE REPRESENTATIVES:
More informationName Class Date. What is ionic bonding? What happens to atoms that gain or lose electrons? What kinds of solids are formed from ionic bonds?
CHAPTER 1 2 Ionic Bonds SECTION Chemical Bonding BEFORE YOU READ After you read this section, you should be able to answer these questions: What is ionic bonding? What happens to atoms that gain or lose
More informationLecture 34: Symmetry Elements
Lecture 34: Symmetry Elements The material in this lecture covers the following in Atkins. 15 Molecular Symmetry The symmetry elements of objects 15.1 Operations and symmetry elements 15.2 Symmetry classification
More informationNew York State Student Learning Objective: Regents Geometry
New York State Student Learning Objective: Regents Geometry All SLOs MUST include the following basic components: Population These are the students assigned to the course section(s) in this SLO all students
More informationBonds. Bond Length. Forces that hold groups of atoms together and make them function as a unit. Bond Energy. Chapter 8. Bonding: General Concepts
Bonds hapter 8 Bonding: General oncepts Forces that hold groups of atoms together and make them function as a unit. Bond Energy Bond Length It is the energy required to break a bond. The distance where
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More information*1. Derive formulas for the area of right triangles and parallelograms by comparing with the area of rectangles.
Students: 1. Students understand and compute volumes and areas of simple objects. *1. Derive formulas for the area of right triangles and parallelograms by comparing with the area of rectangles. Review
More informationExplain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds.
Problem 1 Explain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds. Ionic Bonds Two neutral atoms close to each can undergo an ionization process in order
More informationSection 1.1. Introduction to R n
The Calculus of Functions of Several Variables Section. Introduction to R n Calculus is the study of functional relationships and how related quantities change with each other. In your first exposure to
More information3/5/2014. iclicker Participation Question: A. MgS < AlP < NaCl B. MgS < NaCl < AlP C. NaCl < AlP < MgS D. NaCl < MgS < AlP
Today: Ionic Bonding vs. Covalent Bonding Strengths of Covalent Bonds: Bond Energy Diagrams Bond Polarities: Nonpolar Covalent vs. Polar Covalent vs. Ionic Electronegativity Differences Dipole Moments
More informationCHEMISTRY BONDING REVIEW
Answer the following questions. CHEMISTRY BONDING REVIEW 1. What are the three kinds of bonds which can form between atoms? The three types of Bonds are Covalent, Ionic and Metallic. Name Date Block 2.
More informationPrentice Hall Algebra 2 2011 Correlated to: Colorado P12 Academic Standards for High School Mathematics, Adopted 12/2009
Content Area: Mathematics Grade Level Expectations: High School Standard: Number Sense, Properties, and Operations Understand the structure and properties of our number system. At their most basic level
More information